Modular structure of a robust microporous MOF based on Cu2 paddle-wheels with high CO2 selectivity
Jose M. Seco; David Fairen-Jimenez; Antonio J. Calahorro; Laura Mendez-Linan; Manuel Perez-Mendoza; Nicola Casati; Enrique Colacio; Antonio Rodriguez-Dieguez; Chem.Commun. 49 (2013) 11329–; doi:10.1039/c3cc44193h

data_7110058
_publ_section_title
;
 Modular structure of a robust microporous MOF based on Cu2 paddle-wheels
 with high CO2 selectivity
;
_journal_name_full               Chem.Commun.
_journal_page_first              11329
_journal_paper_doi               10.1039/c3cc44193h
_journal_volume                  49
_journal_year                    2013
_chemical_formula_sum            'C23 H26 Cu2 N2 O8'
_chemical_formula_weight         585.54
_chemical_name_systematic
;
 ?
;
_space_group_IT_number           15
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 104.58(3)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   27.449(18)
_cell_length_b                   13.1546(14)
_cell_length_c                   8.4882(11)
_cell_measurement_temperature    293(2)
_cell_volume                     2966(2)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_diffrn_ambient_pressure         1100000(100000)
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.494
_diffrn_measured_fraction_theta_max 0.494
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi scans'
_diffrn_radiation_monochromator  silicon
_diffrn_radiation_source         synchrotron
_diffrn_radiation_type           synchrotron
_diffrn_radiation_wavelength     0.30969
_diffrn_reflns_av_R_equivalents  0.0916
_diffrn_reflns_av_sigmaI/netI    0.0699
_diffrn_reflns_limit_h_max       21
_diffrn_reflns_limit_h_min       -20
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_l_max       9
_diffrn_reflns_limit_l_min       -9
_diffrn_reflns_number            6303
_diffrn_reflns_theta_full        10.48
_diffrn_reflns_theta_max         10.48
_diffrn_reflns_theta_min         1.73
_exptl_absorpt_coefficient_mu    0.163
_exptl_absorpt_correction_T_max  1.00
_exptl_absorpt_correction_T_min  0.91
_exptl_absorpt_correction_type   sphere
_exptl_crystal_colour            green
_exptl_crystal_density_diffrn    1.311
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             1200
_exptl_crystal_size_max          0.07
_exptl_crystal_size_mid          0.07
_exptl_crystal_size_min          0.02
_refine_diff_density_max         0.511
_refine_diff_density_min         -0.468
_refine_diff_density_rms         0.107
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.118
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     65
_refine_ls_number_reflns         1244
_refine_ls_number_restraints     10
_refine_ls_restrained_S_all      1.116
_refine_ls_R_factor_all          0.1045
_refine_ls_R_factor_gt           0.0797
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.1367P)^2^+11.9420P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2255
_refine_ls_wR_factor_ref         0.2425
_reflns_number_gt                933
_reflns_number_total             1244
_reflns_threshold_expression     >2\s(I)
_cod_data_source_file            c3cc44193h.txt
_cod_data_source_block           anto1p1
_cod_original_sg_symbol_H-M      C2/c
_cod_database_code               7110058